O1 steel also is called DIN 1.2510 and JIS SKS3 steel. High content for manganese, chromium and tungsten in 1.2510 steel composition, that could increase the hardening ability. Then the steel does not need to undergo water quenching. After oil cooling and quenching, the hardness could reach 62HRC. O1 tool steel round bar sheet plate was used widely as a cold work mold steel. It is a great material for the blade, metal molds and etc. O1 steel properties and O1 steel heat treat as below.
1.2510 Steel Characteristics
- It is pre-hardened, texture consistent, high hardenability.
- High cleanliness and excellent polishing performance.
- Good electrical processing properties and texture processing properties.
O1 Steel Application
1.2510 steel is used as a material of tough parts. Such as punches, knock-out pins, cams, and of course, knife blades. And 1.2510 steel is mainly used for short-run tooling for cold forming dies, blanking dies, and cutting tools operating at ambient temperature. Typical applications for O1 tool steel are blanking, forming, and trim dies, gages, slitting cutters and etc.
1.2510 Steel Physical Properties
|Density(hardened to 62 HRC)||7.81 g/cm³||0.282 lb/in³|
|Density(@399°C/ 750°F, hardened to 62 HRC)||7.70 g/cm³||0.278 lb/in³|
|Density(@191°C/ 375°F, hardened to 62 HRC)||7.75 g/cm³||0.280 lb/in³|
O1 Steel Mechanical Properties
|Hardness, Brinell(soft annealed -delivery condition)||190||190|
|Hardness, Rockwell C(tempering temp 300-1200°F)||34.0-64.0||34.0-64.0|
|Elastic modulus(hardened to 62 HRC)||193 GPa||28000 ksi|
|Elastic modulus(@399°C/750°F, hardened to 62 HRC )||172 GPa||25000 ksi|
|Elastic modulus(@191°C/375°F, hardened to 62 HRC)||186 GPa||27000 ksi|
|Compressive yield strength(0.2%, hardened to 50 HRC)||1350 MPa||196000 ksi|
|Compressive yield strength(0.2%, hardened to 55 HRC)||1800 MPa||261000 ksi|
|Compressive yield strength(0.2%, hardened to 60 HRC)||2150 MPa||312000 ksi|
|Compressive yield strength(0.2%, hardened to 62 HRC)||2200 MPa||319000 ksi|
O1 Steel Grade Equivalent Chart
|Standard||ASTM A681||DIN EN ISO 4957||JIS G4404|
O1 Steel Chemical Composition and Equivalent Grades
|EN ISO 4957||0.90-1.05||1.00-1.20||0.03||0.03||0.15-0.35||0.50-0.70||0.05-0.15||0.50-0.70||-|
|JIS G4404||0.90-1.00||0.90-1.20||0.03||0.03||max 0.35||0.50-1.00||-||0.50-1.00||-|
O1 Steel Round Bar Sheet Plate Heat Treatment
Stress Relief of Unhardened Material
Heat slowly to 1250° F. Soak for two hours per inch of thickness at heat. Slow cool (furnace cool if possible) to room temperature.
Ac1: 1350°F Ac3: 1400°F
Ar1: 1295°F Ar3: 1240°F
Heat at a rate not exceeding 400°F per hour (222°C per hour) to 1200-1300°F (649-704°C) and equalize.
Austenitizing (High Heat)
Heat slowly from the preheat to 1475-1500°F (802-816C)
Soak for 30 minutes for the first inch (25.4 mm) of thickness, plus 15 minutes for each additional inch (25.4 mm).
Oil quenching to a temperature no lower than 150-125°F (66-51°C).
O1 steel is prone to quench cracking, especially if there are significant changes in section thickness and sharp internal corners. The oil quenching should be performed so that the heat removal is as uniform as possible in all areas of the part being quenched. Be sure to remove the part from the oil before the temperature drops to ambient temperature. Hot oil at a temperature of 300 to 400°F (149-204°C) is recommended.
Temper immediately after quenching. Do not allow the part to cool below 125°F (51°C). The typical tempering range is 350 – 400°F (177 -204°C). Hold at temperature for 1 hour per inch (25.4 mm) of thickness, 2 hours minimum, then air cool to ambient temperature. To minimize internal stresses in cross sections greater than 3 inches (76.2 mm) and to improve stability in parts that will be EDM’d after heat treatment, a soaking time of 4 to 6 hours at the tempering temperature is strongly recommended.
Refrigeration treatments should typically be performed after the temper, and must be followed by a second temper.
Annealing must be performed after hot working and before re-hardening.
Heat at a rate not exceeding 400°F per hour (222°C per hour) to 1425 -1450°F (802-816°C), and hold at temperature for 1 hour per inch (25.4mm) of maximum thickness; 2 hours minimum. Then cool slowly with the furnace at a rate not exceeding 50°F per hour (28°C per hour) to 1000°F (538°C). Continue cooling to ambient temperature in the furnace or in air. The resultant hardness should be a maximum of 212 HBW.
1.2510 Steel Quality Certificate
Specification: Dia 20-600mm; Length: <5800mm(fit 20ft container); >5800mm, 40ft container
Surface: original black, peeled, machined/turned, polished/ grounded/milled/grinded
Specification: thickness: 10-600mm; width: 30-810mm; length: same as above
Surface: original black, machined/turned, polished/ grounded/milled/grinded
We have our own cutting and processing equipment. Specifications can be cut and customized according to your requirements.
We are a professional special steel stockist and supplier with a high-quality stand for many years. Please contact us for any request of O1/1.2510 steels materials. Songshun Steel always with you.
AISI 6150 steel is an alloy spring steel. It has great mechanical properties......
AISI 52100 steel is the representative of high carbon chromium bearing steel type.
4130 alloy steel has high strength and toughness and the hardenability is high.
It has great mechanical property and processability. And it is great choice for the production of the.....
AISI 5140 steel also can be called JIS Scr440 and DIN 1.7035 steel. It is one of the alloy steel.
AISI O2 steel is the better type compare with the O1 tool steel. Its content of carbon, chromium and tungsten has been raised.
M35 steel is high speed tool steel. After the heat treatment, its hardness, red hardness and wear resistance can be.....
12L14 is a free cutting structural steel. And it is easy to be machined.
1045 carbon steel has a tensile strength is 570-700 MPa and Brinell hardness ranging between 170 and 210.
8620 steel is alloy steel and has good strength and toughness properties. This alloy steel is flexible during....
4340 steel has great machinability, heat treatment stability and impact toughness.
4140 steel is an alloy structural steel with high strength, hardenability, good toughness....
T1 HSS tool steel is the most widely used tungsten type of high speed steel. Its properties are great, has good abrasion, toughness and hardness.
M42 high-speed steel is a cobalt-molybdenum tools steel. The addition of 8% cobalt means that M42 has superior red-hardness when....
AISI M2 high-speed steel has largely replaced T1 in most applications due to its superior properties and advantageous pricing. It is a medium....
According to the AISI classification system, chromium hot-work tool steels are designated as group H steels.
The hardness of A2 steel after heat treatment is higher than SKD11 steel. Its hardness could reach 60-62HRC after....